cutting ductile iron pipe
Post on 28-Mar-2015
Embed Size (px)
FIELD WELDING AND CUTTING DUCTILE IRON PIPE
FIELD WELDING AND CUTTING DUCTILE IRON PIPEBy Richard W. Bonds, P.E. Research and Technical Director
UCTILE IRON PIPE MANUFACTURERS have been successfully welding Ductile Iron pipe for many years and should be consulted on their recommendations for field welding and torch cutting their product. The Ductile Iron Pipe Research Association (DIPRA) does not support indiscriminate field welding of Ductile Iron pipe. However, unforeseen circumstances might require field welding of retainer rings, thrust collars, etc., onto the barrels of Ductile Iron pipe. This manual is intended as a guide for field welding and cutting cement-mortarlined and unlined Ductile Iron pipe. For welding or cutting special lined pipe, consult the pipe manufacturer. The procedures described are intended to be used only by qualified welders having adequate skill and experience in the practice of the appropriate welding and cutting methods for cast ferrous materials. Only such qualified welders should be allowed to field weld and field cut restrained joints for Ductile Iron pipe. Pipe manufacturers recommended procedures shall be followed while exercising reasonable care. Care should also be exercised in the application of the principles contained herein. DIPRA assumes no responsibility and disclaims liability for the design or performance of pipe joints or pipe systems fabricated with this approach. Also, DIPRA assumes no responsibility and disclaims liability for injury or damage to persons or property arising from the use of these procedures.
that have mechanical properties comparable to those of the base iron. As with any base material, the success of welding Ductile Iron depends on suitable equipment, correct procedures, qualified welders, and effective quality control procedures.
Ductile Iron PipeThe first Ductile Iron pipe was cast experimentally in 1948. Years of metallurgical, casting, and quality control refinement followed, and in 1955 Ductile Iron pipe was introduced into the marketplace. Its phenomenal strength and impact resistance compared to Gray Iron, along with many other advantages, created a rapid increase in demand for this product as engineers and utility officials realized that it could be transported, handled, and installed with virtually no damage to the pipe. In service, Ductile Iron pipe showed that expense of repair was practically eliminated. Ductile Iron is usually defined as a Cast Iron with primary graphite in the nodular or spheroidal form. This change in the graphite form is accomplished by adding an alloy, usually magnesium, to molten iron of appropriate composition. Properly treated iron will solidify with the graphite in the form of nodules or spheroids. The distribution and shape of the graphite nodules are set when the metal solidifies in the mold and will remain essentially unchanged during subsequent processing. Because of the mold cooling and rapid iron solidification, the pipe must be annealed (heat treated) to produce the necessary proportion of ferrite that imparts strength, ductility, and impact properties required by specifications for water service. The annealing treatment relieves casting stresses and produces the microstructural transformation that increases the toughness and improves ductility of the
IntroductionWelding is a very important fabrication method in modern industry. If an alloy can be welded successfully, its usefulness is clearly enhanced. Ductile Iron can be welded successfully to produce weldsAs these photomicrographs show, Ductile Iron differs from Gray Iron in that its graphite is spheroidal, or nodular, instead of the flake form found in Gray Iron. Ductiles greater strength, ductility, and toughness are due to this change in microstructure.
Copyright 1998, 1992 by Ductile Iron Pipe Research Association
The annealing treatment for Ductile Iron pipe relieves casting stresses and produces the microstructural transformation that increases the pipes toughness and improves the ductility of the iron while maintaining the required strength.
iron while maintaining the required strength. The effectiveness of the magnesium treatment of the iron as well as the annealing treatment of the pipe is proven by means of physical tests. The types of tests, test frequencies, and acceptance limits that are required are specified in ANSI/AWWA C151/A21.51 Standard, Ductile-Iron Pipe, Centrifugally Cast, for Water. The acceptance test requirements of the ANSI/AWWA C151/A21.51 Ductile Iron Pipe Standard are: 1.Tensile properties of specimens machined from the pipe wall: ultimate strength, 60,000 psi minimum; yield strength, 42,000 psi minimum; elongation, 10 percent minimum. 2.Charpy V-Notch impact strengths on specimens cut from the pipe wall: 7 ft-lb minimum at 70F; 3 ft-lb minimum at -40F. Ferritic Ductile Iron, as compared to Gray Iron, will have about twice the strength as determined by a tensile test, beam test, ring bending test, and bursting test. The tensile elongation and impact strength of Ductile Iron are many times that of Gray Iron.
General Welding of Iron PipesWeldability of Ductile Iron Due to their high carbon content, all cast
irons have a common factor affecting their weldability. During the welding of cast irons, the iron immediately adjacent to the weld metal is heated to its fusion or melting point. After welding, the entire heat-affected zone cools very rapidly. During this heating and cooling, some of the graphitic carbon dissolves and diffuses into the iron, and, as a result, carbides tend to form at the edge of the fusion zone, and high-carbon martensite and bainite tend to form in the remainder of the heat-affected zone. The formation of these hard, brittle microconstituents increases the susceptibility to cracking. The lower surface-to-volume ratio of the nodular graphite in Ductile Iron as compared to that for the flake graphite in Gray Iron results in less carbon dissolution and the formation of fewer carbides and less high-carbon martensite. Also, because of its localized nature, welding produces thermal stresses in the weld area. Ductile Iron pipe, having a predominantly ferritic matrix, is capable of local plastic deformation to accommodate these welding stresses and is therefore better suited to absorb welding stresses than is Gray Iron. Successful welds can be made by minimizing the stress from contraction of the weld metal as it cools, the pick-up of carbon by the weld metal, and by controlling the rate of cooling.
Preparation for Welding The success of any welding operation is affected by how effectively the preparation and cleaning operations are carried out prior to welding. The welding area on the pipe and connecting piece must be untarnished, dry, and grease-free. It has been found that the asphaltic coating on the pipe can most easily be removed with a torch. An alternate method is to wash and wipe the area with a wellsoaked rag containing mineral spirits or other solvents. (Safety precautions must be observed when using flammable materials.) After the asphaltic coating and any grease, etc., have been removed from the weld area, the area should be ground to bright metal to remove all annealing oxide. Also, the corresponding surface of the Ductile Iron or alloy steel connecting piece to be welded should be cleaned and ground to bright metal. A shot-blasted surface alone is not adequate for welding. Weld Joint Design Most weld joint designs commonly used for welding carbon steels are generally suitable for welding Ductile Iron (butt welding is not recommended). Preheating Preheating involves raising the temperature of the base metal in the region to be welded to a predetermined temperature prior to carrying out the welding
process. Preheating may be applied to help prevent cold-cracking, reduce hardness in the heat-affected zone, reduce residual stresses, and reduce distortion. Normally, preheating of Ductile Iron pipe is not necessary and is impractical to do in the field. However, in extreme cold weather one may find it advantageous to warm the pipe weld area with a torch. Shielded Metal-Arc Welding Shielded metal-arc welding is the most common welding process used on Ductile Iron pipe in the field. The equipment necessary for shielded metal-arc welding is as follows: 1.D.C. arc welder using reversed polarity. 2.Suitable welding electrodes. 3.Welding cable, work-piece cable, electrode holder, gloves, shield and protective clothing. Electrodes for metal-arc welding are normally covered with a flux coating. The coating can fulfill the following functions: 1.Stabilize the arc by ionization. 2.Provide protection for the molten metal from the atmosphere by evolution of gases such as carbon dioxide and by hydrogen and also by the formation of a protective slag or flux. 3.Influence the properties of the weld metal by de-oxidation and alloying. 4.Control the arc characteristics. Recommended Electrodes Some electrodes recommended for welding Ductile Iron are the 44- and 55percent nickel-iron electrodes. Consult pipe manufacturer for recommendations. These electrodes provide weld metal strength and toughness properties that are comparable to those of the base iron. The 44- and 55-percent nickel-iron electrodes should be in conformance with class designation AWS A5.15
(ERNi-CI) and (ENiFe-CI) respectively. These electrodes are capable of producing suitable welds without preheating or postheating the pipe or connecting piece. Nickel-iron electrodes are available from most of the leading electrode manufacturers and, although composition with reference to nickel and iron content remains broadly the same, differences in slag-stripping qualities and operation may be found in electrodes obtained from different sources. Two nickel-iron electrod